Research Article  Open Access
S. K. Deb Nath, SungGaun Kim, "Study of the Nanomechanics of CNTs under Tension by Molecular Dynamics Simulation Using Different Potentials", International Scholarly Research Notices, vol. 2014, Article ID 606017, 18 pages, 2014. https://doi.org/10.1155/2014/606017
Study of the Nanomechanics of CNTs under Tension by Molecular Dynamics Simulation Using Different Potentials
Abstract
At four different strain rates, the tensile stress strain relationship of singlewalled 1212 CNT with aspect ratio 9.1 obtained by Rebo potential (Brenner, 1990), Airebo potential (Stuart et al., 2000), and Tersoff potential (Tersoff, 1988) is compared with that of Belytschko et al. (2002) to validate the present model. Five different empirical potentials such as Rebo potential (Brenner, 1990), Rebo potential (Brenner et al., 2002), Inclusion LJ with Rebo potential (Brenner, 1990), Airebo potential (Stuart et al., 2000), and Tersoff potential (Tersoff, 1988) are used to simulate CNT subjected to axial tension differing its geometry at high strain rate. In Rebo potential (Mashreghi and Moshksar, 2010) only bondorder term is used and in Rebo potential (Brenner et al., 2002) torsional term is included with the bondorder term. At high strain rate the obtained stress strain relationships of CNTs subjected to axial tension differing its geometries using five different potentials are compared with the published results and from the comparison of the results, the drawback of the published results and limitations of different potentials are evaluated and the appropriate potential is selected which is the best among all other potentials to study the elastic, elasticplastic properties of different types of CNTs. The present study will help a new direction to get reliable elastic, elasticplastic properties of CNTs at different strain rates. Effects of long range Van der Waals interaction and torsion affect the elastic, elasticplastic properties of CNTs and why these two effects are really needed to consider in bondorder Rebo potential (Brenner, 1990) to get reliable elastic, elasticplastic properties of CNTs is also discussed. Effects of lengthtodiameter ratio, layering of CNTs, and different empirical potentials on the elastic, elasticplastic properties of CNTs are discussed in graphical and tabular forms with published results as a comparative manner to understand the nanomechanics of CNTs under tension using molecular dynamics simulation.
1. Introduction
A variety of new intriguing materials have been discovered and synthesized in the last two decades which have caused phenomenal change in the area of materials science and among them one is the class of carbon compounds referred to fullerene nanotubes. Carbon nanotubes can be made of as rolling up sheets of graphite that are sometimes crapped on each end, with structures that vary depending on the conditions under which they are synthesized. They are singlewalled [1, 2] with diameters as small as about 1 nm or multiwalled [3, 4] with outer diameters ranging from 5 to 350 nm. Since their discovery by Lijima and Lchihashi [1] carbon nanotubes (CNTs) have been the subject of extensive research due to their unique structural and electronic properties that lead to a wide range of potential applications from electronics [5] to mechanical reinforcements in composites [6]. Early studies on the mechanical properties of CNT were carried out considering compression test [7, 8]. Yakobson et al. [7] first investigated the instability of single wall CNT under axial compression, bending, and torsional deformation using continuum shell model. Yakobson et al. [9] studied the behavior of CNTs under a high strain rate using TersoffBrenner’s reactive empirical bondorder (REBO) potential [10, 11].
Sinnott et al. [12] estimated the theoretical Young’s moduli for carbon fibers composed of singlewalled fullerene nanotubes aligned in the direction of the tubule axis. They also investigated a new carbon composite composed of layered nanotubule fibers and diamond and they observed that this composite had a highmodulus, lowdensity material that was quite stable to shear and other distortions. Liew et al. [13] examined the elastic and elasticplastic properties of carbon nanotubes under axial tension using second generation of reactive empirical bondorder potential coupled with the LennardJones potential at high strain rate. In their analysis, plastic regions are not clear because in most of the analysis of CNT it was observed that before breaking the stiffness is the highest which contradicts the reliability of their solution due to the mismanagement of the application of the Van der Waals interactions. They did not minimize CNT structure to reach its minimum energy before applying tensile loading at its both ends. Besides, Liew et al. [13] did not include temperature effect in the theoretical Rebo potential [11] and Van der Waals interaction for analyzing the elastic, elasticplastic properties of CNTs by molecular dynamic simulation. So, the elasticplastic properties obtained by Liew et al. [13] by molecular dynamics simulation are not beyond doubtful quality of solutions. Molecular dynamics simulations of tensile pulling of carbon nanotubes (SWCNTs) (both armchair and Zigzag configurations) were conducted using the Brenner potential to investigate the variation of sixcarbon bond lengths and bond angles of the hexagons in singlewalled carbon nanotubes (SWCNT) as a function of tensile strain [14]. For armchair CNTs, the brittle fracture is observed and the ultimate strength of CNTs is many times to that of CNTS obtained by Liew et al. [13]. The stress strain relationship of armchair CNT using Rebo potential by the tension test in molecular dynamics environment by Agrawal et al. [14] contradicts the elasticplastic region of CNT by Liew et al. [13] although in his analysis Van der Waals interactions are absent. Wang and Vijayaraghavan [15] studied the buckling characteristics of several curved forms of singlewalled carbon nanotubes by molecular dynamics simulations using Rebo potential [11] and Van der Waals interaction. Tserpes and Papanikos [16] proposed a threedimensional finite element model for armchair, Zigzag, and chiral singlewalled carbon nanotubes which is based on the assumption that carbon nanotubes, when subjected to loading, behave like spaceframe structures. The bonds between carbon atoms are considered as connecting load carrying members while the carbon atoms as joints of the members [16]. To create the FE models, nodes are placed at the locations of carbon atoms and the bonds between them are modeled using threedimensional elastic beam elements and the elastic properties of armchair, Zigzag, and chiral singlewalled carbon nanotubes are obtained which are compared with those of experimental results to verify the FE model [16]. SalvetatDelmotte and Rubio [17] concluded that CNTs have indeed a great potential as reinforcing elements for composites. Coto et al. [18] studied the effect of carboxylation on axial Young’s modulus of carbon nanotubes using molecular dynamics simulation. COMPASS force field is used to model the interatomic interactions in single wall (SWCNT) and multiwall carbon (MWCNT) with different amount of –COOH group attached to their surfaces [18]. Mashreghi and Moshksar [19] determined the structural parameters of several armchair singlewalled carbon nanotubes such as potential energy as a function of bond length and bond angles, respectively, using molecular dynamics simulations. Tang et al. [20] synthesized carbon nanotube polymer composites mixing carbon nanotubes and high density polyethylene by using the melt processing method and they observed that the stiffness, peak load, and work to failure for the composite films increase with the increase of MWCNT content. Sammalkorpi et al. [21] studied how the Young’s modulus and tensile strength of nanotubes depends on defects employing molecular dynamics simulation and continuum theory. The Young’s modulus of nanotubes with defects will essentially be the same unless the number of vacancy concentration is extremely high [21]. On the other hand, the tensile strength will substantially drop due to the quasionedimensional atomic structure of SWNTs already if a single vacancy is present; the tensile strength of a SWNT is governed by the weakest segment of the tube [21]. Wang et al. [22] observed that composites showed higher mechanical properties such as the Young’s modulus and tensile strength of the SWNT/epoxy composite rise with the increase of SWNT concentration. The Young’s modulus and yield strength have been doubled and quadrupled for composites with, respectively, 1 and 4 wt% of nanotubes compared to the pure resin matrix samples [23]. A recent research illustrates qualitative relationship between Young’s modulus of a CNT and the amount of disorder in the atomic structure of the walls [24]. Lin and Chen [25] evaluated the effective mechanical properties of CNTbased composites using a 3D nanoscale representative volume element based continuum mechanics and the finite element method. HernándezPérez and Avilés [26] investigated the influence of the interphase on the effective properties of carbon nanotube composites using finite element analysis and elasticity solutions for representative volume elements. Micro Pt wire exhibits higher strength as compared to its bulk due to decreasing size which is observed from the experimental study of bending test of Pt microwire with the help of finite element analysis [27]. In the very short range of diameters in Au nanowires, Young's modulus and yield strength increase with the decreasing of their diameters which are clearly observed in the bending and tension test of Au nanowires by molecular dynamics simulations [28]. Due to having small sizes of diameters in CNTs and as a result of increasing their surface energy, their strength and stiffness are many times to those of their conventional bulk materials which are made of C elements.
Due to having high stiffness and light weight, CNT is a promising candidate in nanocomposites to increase their strength and stiffness. Nowadays people are concentrating to evaluate the actual elastic, elasticplastic properties of CNTs experimentally and theoretically. But handling CNT in experimental way is a difficult task and the obtained mechanical properties by the experimental way are beyond actual quantitative measures. To obtain the actual quantitative mechanical properties, theoretical approach is only an alternative approach. Researchers are trying to study CNT by quantum ab initio calculations at a very small scale and on the other hand classical molecular dynamics based on empirical potentials are being used to study large size CNT. Besides, very recently, people are trying to study CNTs using finite element and finite volume approach considering continuum approach. Classical molecular dynamics are the only reliable method to get reliable mechanical properties of CNTs, but it depends on the potentials. There are different potentials [10, 11, 29, 31] which are being widely used to obtain elastic, elasticplastic properties of CNT. To predict actual elasticplastic and fracture region, selections of good potentials are necessary. In most of the studies, temperature effect is not included which is beyond practical condition. Firstly the elastic, elasticplastic response of singlewalled 1212 CNTs with aspect ratio 9.1 subjected to a uniform axial loading at its both ends at four different strain rates obtained by Rebo potential [11], Airebo potential [29], and Tersoff potential [10] is compared with that of Belytschko et al. [30] to validate the present model. In the present study, we study the mechanical behaviors of CNTs subjected to a uniform tensile load at its opposite ends at high strain rate using five different potentials by molecular dynamics simulation as a comparative manner with the existing published results and the limitations of the published results as well as our results obtained by different potentials are highlighted and from our analysis we try to select appropriate potential which can give more accurate elastic, elasticplastic response of CNTs at different strain rates. Besides, effects of usual parameters lengthtodiameter ratio, layering of CNTs on the elastic, elasticplastic properties of CNTs are shown by figures and tables. We try to establish the superiority of the present technique and results of CNTs.
2. Simulation Procedure
At four different strain rates such as very low strain rate (stretching velocity at both ends of CNTs is 0.09 m/s), low strain rate (stretching velocity at both ends of CNTs is 0.5 m/s), moderate strain rate (stretching velocity at both ends of CNTs is 5 m/s), and high strain rate (stretching velocity at both ends of CNTs is 20 m/s), the stress strain relationship of singlewalled 1212 CNT with aspect ratio 9.1 subjected to uniform tensile load obtained by Rebo potential [11], Airebo potential [29], and Tersoff potential [10] is compared with that of Belytschko et al. [30] to validate the model. To study the elastic, elasticplastic properties of CNT, we need its stress strain relationship up to its fracture. In this study, we also simulate singlewalled 1010, 1212 CNTs; doublewalled (5,5), 1010 CNTs; threewalled (5,5), 1010 and 1515 CNTs; fourwalled (5,5), 1010, 1515, and 2020 CNTs using molecular dynamics simulation considering five different potentials such as Tersoff [10], Rebo potential [11], Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29] at high strain rate. Firstly the CNT structure is minimized to get its minimum energy using different potentials before applying velocity to two groups of atoms at both ends of CNTs for all strain rates. At high strain rate tension test is carried out applying a constant velocity 20 m/s at some atoms of both ends of the CNT in opposite directions by molecular dynamics simulation. Before applying velocity, the total force on some grouped atoms at both ends of the CNT is kept null so that extra force is not counted during stress strain relationship. Force is counted after applying velocity to a group of atoms at both end of the CNT. And the number of atoms in each group is kept equal. In the microcanonical ensemble molecular dynamics simulations of CNTs, the strain is computed by in which and are the initial and current length of CNTs, respectively, and the stress is obtained by . The axial force is obtained by summing the interatomic force for the atoms at the end of CNTs and the crosssectional area is , where is the diameter of the CNT and is the thickness of the CNT that is taken as nm for a 1010 singlewalled CNT, nm for a twowalled (5,5) and 1010 CNT, nm for a threewalled (5,5), 1010, and 1515 CNT, and nm for a fourwalled (5,5), 1010, 1515, and 2020 CNT. ratio of CNTs is considered as 9.1 and 4.5, respectively, in the present study. Used time step is 0.001 ps and the whole simulation is considered at a temperature 300 K. Using NVT canonical ensemble, temperature is controlled. Details of the used empirical potentials in molecular dynamics simulation of CNTs are discussed in the following sections for clear understanding of the readers. Due to absence of long range Van der Waals interactions and torsional effects in Tersoff potential [10] and Rebo potential [11], Rebo potential [31], and Inclusion LJ in Rebo potential [10], there is possibility of having some inaccuracies of the elasticplastic properties of CNT when the simulation is carried out considering Tersoff potential [10], Rebo potential [11], Rebo potential [31], and Inclusion LJ with Rebo potential [11].
3. Theoretical Formulations
3.1. Tersoff Potential [10]
The energy , as a function of the atomic coordinates by Tersoff [10], is taken to be Here is the total energy of the system, which is decomposed for convenience into a site energy and a bond energy : The indices and run over the atoms of the system, and is the distance from atom to . The function represents a repulsive pair potential, which includes the orthogonalization energy when atomic wave functions overlap, and represents an attractive pair potential associated with bonding: The extra term is merely a smooth cutoff function, to limit the range of the potential, since for many applications short ranged functions permit a tremendous reduction in computational effort.
Here the cutoff function is simply taken as where represents a measure of the bond order and is for now assumed to be a monotonically decreasing function of the coordination of atoms and . Details of refer to Tersoff [10].
3.2. Rebo Potential [11]
The binding energy for the hydrocarbon potential is given as a sum over bounds as where the repulsive and attractive pair terms are given by Here, is the distance between th and th atoms, is a bondorder term, and and are functions of . For more details of these terms, refer to Brenner et al. [10, 11].
3.3. Airebo Potential [29]
Stuart et al. [29] developed a reactive potential for hydrocarbons with intermolecular interactions. With the adaptive treatment of dispersion, intermolecular repulsion, and torsional interactions, the entire energy is given by the expression The REBO interaction is based on the form proposed by Tersoff [10]: in which repulsive and attractive contributions are combined in a ratio determined by the bonding term .
The repulsive term has the form used by Brenner et al. [11, 31]: where the parameters , , and depend on the atom types and . Values for these and all other potential parameters are given in Table II in [29]. The term is a bondweighing factor, which switches off the REBO interactions when the atom pairs exceed typical bonding distances. The switching function takes the form where the switching region for each type of bond is given by a scaling function The attractive pair interaction in (8) is given by a triple exponential, which is switched off smoothly for nonshortranged interactions through the use of bond weight. The term in (8) specifies the bond order for the interaction between and : This term is only roughly equivalent to the usual chemical concept of a bond order and is simply a means of modifying the strength of a bond due to changes in the local environment.
The principal contribution to is the covalent bond interaction, given by the terms and : The penalty function imposes a cost on bonds that are too close to one another. Its functional form is a fifthorder spline. When the central atom is a carbon, the spline also depends on the local coordination number, defined as the sum of the carbononly and hydrogenonly coordination numbers. is a function of and . counts a carbononly coordination number, with representing a Kronecker delta. The hydrogenonly coordination number is defined similarly. Using this coordination number, the anglebending penalty function switches smoothly between a form appropriate for covalent compounds with low coordination and another form suitable for highly coordinated bulk materials: At intermediate value of , the switching function provides for a smooth transition, with given by (11) and the scaling function given by The term is added to improve the potential energy surface for abstraction of hydrogen atoms from hydrocarbons, with where represents the Kronecker delta for atom types and . The term is a twodimensional cubic spline [32] in and , whose coefficients are chosen to reproduce the values of . These terms are included in the REBO model to give accurate bond energies for small hydrocarbons. Although most REBO parameters were not modified in developing the AIREBO model, the values were modified at two points to counteract the additional torsion energies in the AIREBO potential for unsaturated systems such as ethylene and graphite. In addition to the bonding interactions given by (15), the REBO potential also includes contributions to the bond order from radial and conjugation effects. These enter the potential through the term, which is a threedimensional cubic spline in the variables , , and . The indices and are the coordination numbers defined in (16), and is a local measure of conjugation in the  bond: with specifying the range of coordination numbers under which a bond is assumed to be part of a radical or conjugated network: The remaining contribution to the bondorder is : The bondweighting function is The scaling function is The LJ contribution to the  pair energy is includes the traditional LJ term modified by several sets of switching functions. The switching function is Both have continuous first derivatives at the switching region boundaries.
Below a certain separation distance , the magnitude of the LJ term depends on the bonding environment. The gradual exclusion of LJ interactions as changes is controlled by the , scaling function, At intermolecular distances, the LJ interaction is included only if there is no significant bonding interaction between two atoms, as specified by switch, And if the atoms and are not connected by two or fewer intermediate atoms, this latter switch is controlled by bond weights,
The torsional potential for the dihedral angle determined by atoms , , , and is controlled by the term where
4. Results and Discussion
At different strain rates we simulate CNTs subjected to a uniform axial loading at its both ends using Tersoff potential [10], Rebo potential [11], and Airebo potential [29] to understand the effect of strain rates on their potential energy and elastic, elasticplastic properties. To understand the effect of Van der Waals interaction and torsion with bondorder potential per atom potential energy with strain of singlewalled 1212 CNTs subjected to a uniform tension at their both ends obtained by different potentials are compared to each other. At high strain rate, we simulate CNTs subjected to an axial tension at their both ends using five different potentials such as Tersoff potential [10], Rebo potential [11], Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29] to study the effect of potentials on their elastic, elasticplastic properties. Tersoff potential [10] and Rebo potential [11] are bondorder potential by short range cutoff functions. Out of the cutoff distance, carbon atoms in CNT in different planes and layers do not interact although they experience weak Van der Waals interaction. For nonbonded atoms, although the Van der Waals attraction and repulsion exhibit at a short distance but for the bonded atoms, these Van der Waals attraction and repulsion occur at a long distance. When bondorder potential is used, torsional term must be included to get higher accuracy of the solution because during simulation position of atoms changes due to interacting forces among bonded atoms and bond experiences some angular displacement. Stuart et al. [29] introduced long range Van der Waals and torsional terms in Rebo potential [11] and obtained elastic constants, bond energy, vacancy formation energy, enthalpy of carbon in diamond, and graphite structures using Rebo potential [11] and modified Rebo potential, that is, Airebo potential [29], and compared their results obtained by Airebo potential [29] and Rebo potential [11] with experimental results. The results obtained by Airebo potential [29] show better agreement than that of Rebo potential [11] with experimental results. From the study of diamond and graphite structure by Stuart et al. [29], it is clear that Airebo potential [29] is more suitable for getting highly accurate solution of C, H structures than that of Rebo potential [11]. Firstly we obtain per atom potential energy of a singlewalled 1212 CNT as a function of axial strain at a very low strain rate using three different potentials such as Airebo potential [29], Rebo potential [11], and Tersoff potential [10] to understand the effect of Van der Waals interaction and torsional effects on bondorder potential whose effects are reflected in the elastic, elasticplastic properties of CNTs. We obtain the stress strain relationship of a singlewalled 1212 CNT subjected to a uniaxial loading by molecular dynamics simulation using three different potentials at four different strain rates, that is, from very low strain rate to high strain rate, and compare these with that obtained by Belytschko et al. [30] to get reliable potential for studying the mechanics of CNTs. Effects of strain rates on the elastic, elasticplastic properties of a singlewalled 1212 CNT subjected to an axial loading using different potentials are investigated. For very low to high strain rates, a suitable potential is selected for the study of nanomechanics of CNTs from the comparative study of per atom potential energy and tensile stress as a function of axial strain using three different potentials with those of published results. To understand the nanomechanics of singlewalled, doublewalled, threewalled, and fourwalled CNTs at high strain rate, five different potentials are also used which are Rebo potential [11], Rebo potential [31], Airebo potential [29], Tersoff potential [10], and Inclusion LJ in Rebo potential [11]. In Rebo potential [11] only bondorder term is included. In Rebo potential [31] torsion term is added with bondorder term. In Airebo potential [29] Van der Waals interaction and torsional terms are added with bondorder term. In Tersoff potential [10], only bond order is added. In Inclusion LJ in Rebo potential [11], Van der Waals interaction is added with bondorder term. Effects of layering and aspect ratio on the elastic, elasticplastic properties of CNTs are studied at high strain rate considering five different potentials as comparative manners with those of published results. We compare the elastic, elasticplastic properties of different types of CNTs subjected to a tensile load at its opposite end at a high strain rate using five different potentials with that of Liew et al. [13]. Young’s modulus of CNTs is obtained from the slope of the stress strain relationship of CNTs till 5% strain. Yield strength and yield strain of CNTs are measured from a point of the stress strain curve where its slope is the lowest. Ultimate strength and ultimate strain of CNTs are measured from a point of stress strain curve where the stress is the highest. Poisson’s ratio of CNTs is calculated considering the change of its diameter and length just before fracture using the ratio of lateral to longitudinal strain. Besides, we present the elastic, elasticplastic properties of CNTs at high strain rate using different potentials with the published results as a tabular form. We also obtain Young’s modulus, yield strength, yield strain, ultimate strength, and ultimate strain of singlewalled, doublewalled, threewalled, and fourwalled CNTs from the axial stress strain relationships of different types of CNTs using different potentials by molecular dynamics simulation and present in tabular form.
Figure 1 presents the original and final physical configuration just before breaking of a singlewalled 1212 CNT having lengthtodiameter ratio 4.51 using Airebo potential [29]. Figure 2 illustrates per atom potential energy of a singlewalled 1212 CNT with aspect ratio 9.1 as a function of strain at a very low strain rate (stretching velocity at both ends of a CNT is 0.09 m/s) obtained by Rebo potential [11], Airebo potential [29], and Tersoff potential [10] as a comparative manner. From Figure 2, it is clearly observed that per atom potential energy of CNTs obtained by Tersoff potential is the lowest, per atom potential energy of CNTs obtained by Rebo potential [11] is the highest, and per atom potential energy obtained by Airebo potential [29] remains in between them due to addition of Van der Waals and torsional interactions with bondorder term in Airebo potential [29]. Although the slope of per atom potential energy as a function of strain for Rebo potential [11] and Airebo potential [29] is almost the same, the slope of per atom potential energy as a function of axial strain of singlewalled 1212 CNTs obtained by Tersoff potential [10] is higher than that of Rebo potential [11] and Airebo potential [29]. From Figure 2, it is observed that fracture strain of a singlewalled 1212 CNT obtained by Rebo potential [11] and Airebo potential [29] is almost the same, but fracture strain of singlewalled 1212 CNTs obtained by Tersoff potential [10] is the lowest.
(a)
(b)
Figure 3 illustrates the comparative study of the tensile stress strain relationship of singlewalled 1212 CNTs subjected to an axial tension using Rebo potential [11], Airebo potential [29], and Tersoff potential [10] at four different strain rates with that of Belytschko et al. [30]. From Figure 3(a), it is observed that the tensile stress strain relationships of singlewalled 1212 CNTs obtained by Rebo potential [11] and Airebo potential [29] at a very small strain rate (stretching velocity of both ends of CNTs is 0.09 m/s) are very close to that of singlewalled 1212 CNTs by Belytschko et al. [30] but the tensile stress strain relationship obtained by Tersoff potential [10] deviates a large extent from that of Belytschko et al. [30]. From Figure 3(b), it is observed that tensile stress strain relationship of a singlewalled 1212 CNT obtained by Rebo potential [11] and Airebo potential [29] at a small strain rate (stretching velocity at both ends of CNTs is 0.5 m/s) is almost the same and up to yield strength and the tensile stress strain relationship obtained by Rebo potential [11] and Airebo potential [29] matches with that of Belytschko et al. [30] but after yielding, the tensile stress strain relationship of a singlewalled 1212 CNT obtained by Rebo potential [11] and Airebo potential [29] disagrees with that of Belytschko et al. [30]. At a very low (stretching velocity at both ends of CNTs is 0.09 m/s) and low strain (stretching velocity at both ends of CNTs is 0.5 m/s) rate, the slope of stress strain relationship obtained by Tersoff potential is higher than that of Rebo potential [11], Airebo potential [29], and Belytschko et al. [30] because decreasing rate of per atom potential energy of a singlewalled 1212 CNT with axial strain obtained by Tersoff potential is higher than that of Rebo potential [11] and Airebo potential [29] as shown in Figure 2. Ultimate stress and strain of singlewalled 1212 CNT obtained by Rebo potential [11] and Airebo potential [29] are higher than that of Belyschko et al. [30] when the stretching velocity at both ends of CNTs is 0.5 m/s. From Figure 3(c), it is observed that ultimate strength and strain of a singlewalled 1212 CNT at moderate strain rate (stretching velocity at both ends of CNTs is 5 m/s) obtained by Rebo potential [11] are higher than those of Airebo potential [29] because at moderate strain rate Van der Waals and torsional effect decrease per atom potential energy of CNTs with strain for which it takes less strain and time to reach the lowest per atom potential energy for fracture but for fracture of CNTs, opposite phenomenon is observed when tension test of a CNT is carried out using Rebo potential [11] at moderate strain rate. At high strain rate the deviation between ultimate strength and strain of singlewalled 1212 CNTs obtained by Rebo potential [11] and Airebo potential [29] is higher than that of moderate strain rate. At moderate and high strain rate ultimate strength of singlewalled 1212 CNTs obtained by Airebo potential [29] is closer to that of Belytschko et al. [30] than that of Rebo potential [11]. In all strain rates, the slope of the stress strain relationship of a singlewalled 1212 CNT obtained by Tersoff potential [10] is higher than that of Rebo potential [11], Airebo potential [29], and Belytschko et al. [30]. As at very low strain rate the stress strain relationship of a singlewalled 1212 CNT subjected to axial loading obtained by Rebo potential [11] and Airebo potential [29] is very close to that of Belytschko et al. [30], Airebo potential [29] and Rebo potential [11] are suitable for the study of nanomechanics of CNTs at a very low strain rate. At a very low strain rate per atom potential energy with strain of a singlewalled 1212 CNT obtained Airebo potential [29] is more accurate than that of Rebo potential [11] because Stuart et al. [29] observed that the vacancy formation energy, bond energy, and enthalpy of graphite and diamond by Airebo potential [29] is closer to those of experimental result than those obtained by Rebo potential [11]. At moderate and high strain rates Airebo potential [29] will give more accurate per atom potential energy and elastic, elasticplastic response of CNTs during loading till fracture than those of other potentials because each bonded atom experiences Van der Waals interaction and torsional effect during loading and these two terms are not included in the rest of other potentials together.
(a)
(b)
(c)
(d)
Figure 4 describes the stress strain relationship of a singlewalled 1212 CNT having lengthtodiameter ratio, 9.1, subjected to uniform tension at its opposite ends using Airebo potential [29] by molecular dynamics simulation at high strain rate (stretching velocity at both ends of CNTs is 20 m/s). The stress strain relationship curve gives three onset cutoff diameters, where the elastic, elasticplastic properties change suddenly. In Figure 4, the slope of the curve at a certain range is constant; that is, the stiffness of the CNT remains constant and then the slope of the stress strain relationships of the CNT gradually decreases to a zero value; that is, the stiffness of the CNT gradually decreases and when the diameter of the CNT suddenly drops, the slope of the stress strain curve becomes zero and this is the phase change of CNT due to strain hardening and decreasing its diameter suddenly enhances its stiffness to a greater extent till fracture.
Figures 5(a) and 5(b) illustrate the effect of different potentials on per atom potential energy and per atom total energy of CNTs as a function of strain with the tensile load at their both ends by molecular dynamic simulation at high strain rate. Per atom potential energy of loaded CNTs at a specific strain before fracture obtained by Rebo potential [11] is higher than that obtained by Airebo potential [29] as shown in Figure 5(a) due to the absence of the torsional and Van der Waals interaction in Rebo potential [11] and the fracture strain of CNTs obtained by Rebo potential [11] is higher than that of Airebo potential [29] although the per atom potential energy of CNTs during fracture obtained by Rebo potential [11] and Airebo potential [29] is almost the same. As the slope of per atom potential energy as a function of axial strain of loaded CNTs obtained by Rebo potential [11] and Airebo potential [29] is nearly the same and fracture strain of CNTs obtained by Rebo potential [11] considering per atom potential energy is higher than that of Airebo potential [29], the slope of the stress strain relationship of CNTs obtained by Rebo potential [11] and Airebo potential [29] should be the same and ultimate fracture strength of CNTs obtained by Rebo potential [11] should be higher than that of Airebo potential [29]. Although Tersoff potential [10] is also a bondorder potential like Rebo potential [11], the slope of per atom potential energy of CNTs as a function of strain obtained by Tersoff potential [10] is the highest among those of other potentials which means the slope of the stress strain of loaded CNTs obtained by Tersoff potential [10] should be higher than that of other potentials. From Figure 5(a) it is clear that ultimate strength of CNTs obtained by Tersoff potential [10] should be the lowest of all other potentials. Figure 5(b) illustrates per atom total energy as a function of strain of CNTs obtained by five different potentials and after fracture per atom total energy of CNTs obtained by these potential decreases a little amount due to its increased kinetic energy. Effect of kinetic energy on per atom total energy of CNTs obtained by all of the mentioned potentials is small.
(a)
(b)
Liew et al. [13] obtained tensile stress strain relationship of singlewalled, doublewalled, threewalled, and fourwalled CNTs with aspect ratios 9.1 and 4.51, respectively, using Rebo potential [11] with Van der Waals interaction without minimizing the initial configuration of CNTs before applying tensile loading at high strain rate (stretching velocity at both ends of the CNTs is 20 m/s). Before loading CNTs, it remains in minimized energy level. So to get accurate elastic, elasticplastic response of CNTs we should minimize energy before applying loading because after minimization of energy applying potentials in molecular dynamics simulation, the position of C atoms changes and little changes are observed in shapes of CNTs. Besides, Agrawal et al. [14] studied elastic, elasticplastic response of single wall CNTs subjected to a uniform axial loading varying C–C bond length and bond angle at high strain rate using only bondorder Rebo potential [11]. In the present simulation of CNTs, we minimize different types of CNTs with aspect ratios 9.1 and 4.51, respectively, before loading using five different potentials and then apply load at its both ends (stretching velocity at both ends of CNTs is 20 m/s) like Liew et al. [13] and Agrawal et al. [14]. We compare the tensile stress strain relationships of singlewalled CNTs obtained by us using Rebo potential [11], Rebo potential [31], Airebo potential [29], Inclusion LJ with Rebo potential [11], and Tersoff potential [10] with those of Agrawal et al. [14] and Liew et al. [13]. Besides, we compare the tensile stress strain relationships of doublewalled, threewalled, and fourwalled CNTs obtained by us using Rebo potential [11], Rebo potential [31], Airebo potential [29], Inclusion LJ with Rebo potential [11], and Tersoff potential [10] with those of Liew et al. [13]. From the comparative studies, we try to obtain accurate tensile stress strain relationships of different types of CNTs and suitable potential for finding more accurate elastic, elasticplastic response of CNTs during loading at high strain rate. Figures 6(a) and 6(b) illustrate the tensile stress strain relationship of singlewalled 1212 CNT having length diameter ratios 9.1 and 4.5, respectively, by five different potentials with two published results as a comparative manner at high strain rate (stretching velocity at both ends of CNTs is 20 m/s). The nature of the elasticplastic region obtained by Agrawal et al. [14] is totally different from that of Liew et al. [13]. The elasticplastic region obtained by the present five different potentials agrees well with that of Agrawal et al. [14] although Agrawal et al. [14] solved the CNT problem using Rebo potential [11]. On the other hand Liew et al. [13] solved the CNT problem using Rebo potential including Van der Waals interactions and we also solved the CNT problem using Airebo potential [29], Inclusion LJ with Rebo potential [11] in which Airebo potential [11] consist of long range Van der Waals interaction and torsional effect of bond as well as Inclusion LJ with Rebo potential [11] consist of Rebo potential [11] and Van der Waals interaction. The elasticplastic region of CNT obtained by Airebo potential agrees well with that of Agrawal et al. [14] and the ultimate strength of CNT obtained by Agrawalet al. [14] is higher from that of Airebo potential [29] because they did not consider Van der Waals interactions and torsional effect. From the comparative study, it is clear that the elastic, elasticplastic properties of CNT obtained by Airebo potential [29] are more reliable and accurate. The elastic, elasticplastic response of CNT by Liew et al. [13] does not agree well with other results due to lack of minimization of CNT structure before loading. Besides, the magnitude of the potential depth for Van der Waals interaction as shown in Table 1 is nearly two times that of ours in Airebo potential [29] and it is another reason to deviate the stress strain relationship of singlewalled 1212 CNTs by Liew et al. [13] from that of ours and Agrawal et al. [14]. Effects of Van der Waals interaction and torsional effect on the per atom potential energy with strain, stress strain relationship of CNTs subjected to uniform tension at high strain rate are clearly observed in Figures 5 and 6. Figures 7(a) and 7(b) illustrate the tensile stress as a function of axial strain of a singlewalled 1010 CNT with lengthtodiameter ratios 9.1 and 4.51, respectively, using five different potentials with the published results by Liew et al. [13]. Up to elastic region, the stress strain relationship obtained by five different potentials agrees well with Liew et al. [13] but in the elasticplastic region, the shapes of the curves of the stress strain relationship of CNT by us for five different potentials are different from that of Liew et al. [13] which contradicts the reliability of the stress strain relationship obtained by Liew et al. [13] because the stress strain relationship of CNTs for five different potentials shows three onset cutoff which ensure sudden change in diameter of the CNT which is also reflected in the recent published results by Agrawal et al. [14] and Sammalkorpi et al. [21]. Variations of stress strain relationships of singlewalled CNTs are observed if lengthtodiameter ratio and diameter of CNTs are varied as shown in Figures 6 and 7.
(a)
(b)
(a)
(b)
From Figures 8(a) and 8(b), it is observed that the stress strain relationship of a doublewalled CNT differs for five different potentials although the trends of the shape of the stress strain relationship are similar and the elastic range, the stress strain relationship obtained by five different potentials are nearly equal to that of Liew et al. [13]. In the elasticplastic range of doublewalled CNTs, our results obtained by five different potentials disagree with that of CNTs obtained by Liew et al. [13]. Figures 9 and 10 illustrate the same stress strain relationship of threewalled and fourwalled CNTs in two aspect ratios 9.1 and 4.5 using five different potentials with the published results by Liew et al. [13] as a comparative manner at high strain rate; the stress strain relationship in the elastic range of threewalled and fourwalled CNTs obtained by five different potentials agrees with that of Liew et al. [13], but the stress strain relationship in the elasticplastic range of threewalled and fourwalled CNTs obtained by five different potentials does not agree with that of Liew et al. [13]. Among the stress strain relationships obtained by Tersoff potential [10], Rebo potential [11], Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29], there is the highest reliability in the stress strain relationship obtained by using Airebo potential [29] because this potential includes long range Van der Waals interaction and torsional effect of bonds with Rebo potential [11]. Naturally every bonded atom experiences weak Van der Waals interaction after a certain distance; when bonded atom displaces its position, there is some angular displacement for which C–C bonds of CNTs experience torsion. At very low strain range the stress strain relationship of a singlewalled 1212 CNT obtained by Rebo potential [11] and Airebo potential [29] agrees well with that of Belytschko et al. [30]. Although at very low strain range, the effects of Van der Waals interaction and torsional effect on the elastic, elasticplastic response are negligible, at moderate and high strain rate, the effects of Van der Waals interaction and torsion effect play important roles which are observed in the graphical results of stress strain relationships of CNTs during loading (see Figures 3 and 6–10). Effects of Van der Waals interaction and torsional effects on per atom potential energy of CNTs during tension at different strain rates are observed (see Figures 2 and 5). Effects of layering on the stress strain relationship of CNTs subjected to tensile load at a high strain rate are also observed as shown in Figures 8 to 10. Effects of Van der Waals interaction and torsion on the stress strain relationships of doublewalled, threewalled, and fourwalled CNT are observed from their comparative study of those of Rebo potential [11], Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29] as observed in Figures 8 to 10. Figure 11 illustrates the physical configuration of fourwalled CNTs at different steps till fracture. In the outer layer of a fourwalled CNT, how 5775 defects generate during fracture which are reflected in Figure 11(c).
(a)
(b)
(a)
(b)
(a)
(b)
(a)
(b)
(c)
Table 2 lists the computed Young’s modulus, poison’s ration, yield strength, ultimate strength, yield strain, and ultimate strain of singlewalled 1212 and 1010 CNTs with lengthtodiameter ratios equal to 9.1 and 4.51, respectively, using five different potentials. Young’s modulus, yield strength, and yield strain of singlewalled 1212 CNTs having aspect ratio 9.1 obtained by five different potentials separately are lower than those of aspect ratio 4.51, but the opposite phenomenon is observed for its ultimate strength because per atom potential energy change with strain is higher for CNTs with lower aspect ratio than from its higher aspect ratio. Young’s modulus and yield strength of a singlewalled 1010 CNT having aspect ratio 9.1 obtained by Rebo potential [11], Rebo potential [31], and Airebo potential [29] are lower than those of aspect ratio 4.51; on the other hand, ultimate strength and strain having aspect ratio 9.1 obtained by Rebo potential [11], Rebo potential [31], Airebo potential [29], Inclusion LJ with Rebo potential [11], and Tersoff potential [10] are lower than those of aspect ratio 4.51, separately. Per atom potential energy with strain is dramatically changed due to change of aspect ratio of CNTs which change the slope of stress strain curve of CNTs subjected to a tensile load using different potentials and for which effects of aspect ratio are observed on the elastic, elasticplastic properties of CNTs. From Table 2, it is observed that Young’s modulus, yield strength, yield strain, ultimate strength, and ultimate strain of 1212 singlewalled CNTs with the same aspect ratio differ from those of singlewalled 1010 CNTs due to the size effect in diameters because diameter of singlewalled 1212 CNT is higher than that of singlewalled 1010 CNTs. Effects of different potentials on Young’s modulus, yield strength, yield strain, ultimate strength, ultimate strain, and poison’s ration of singlewalled 1212 and 1010 CNTs are also observed in the tabular results.

Table 3 lists the computed Young’s modulus, yield strength, ultimate strength, yield strain, and ultimate strain of doublewalled, threewalled, and fourwalled CNTs with lengthtodiameter ratios 9.1 and 4.51, respectively, using five different potentials with the published results. Young’s moduli of doublewalled CNT having aspect ratio 9.1 obtained by Airebo potential [29], Rebo potential [11], Rebo potential [31], and Inclusion LJ with Rebo potential [11] are lower than those of aspect ratio 4.51, separately, but yield strengths of a doublewalled CNT having aspect ratio 4.51 using Rebo potential [11], Rebo potential [31], Airebo potential [29], Inclusion LJ with Rebo potential [11], and Tersoff potential [10] are higher than those of aspect ratio 9.51, separately. Yield strains, ultimate strengths, and ultimate strains of doublewalled CNTs having aspect ratio 4.51 using Rebo potential [11], Rebo potential [31], and Airebo potential [29] are lower than those of aspect ratio 9.1. Although Young’s modulus of CNTs with aspect ratio 9.1 obtained by Tersoff potential is higher than that of aspect ratio 4.51, for yield strength, yield strain, ultimate strength, and ultimate strain, the opposite phenomenon is observed. Young’s moduli, yield strengths, and ultimate strengths of threewalled CNT with aspect ratio 9.1 obtained by all potentials mentioned in the Table 3 are higher than those of aspect ratio 4.51, separately. Yield strain and ultimate strain of threewalled CNTs obtained by Rebo potential [11], Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29] mentioned in Table 3 also show the effect of aspect ratio of CNTs. Young’s moduli, yield strengths, ultimate strengths of fourwalled CNT with aspect ratio 4.51 obtained by all potentials mentioned in the Table 3 are higher than those of aspect ratio 9.1, separately. There are also observed effects of aspect ratio on the yield strains and yield strengths of fourwalled CNTs obtained by all potentials mentioned in Table 3. From Table 3, it is clearly observed that Young’s moduli, yield strengths, yield strains, ultimate strengths, and ultimate strains of doublewalled, threewalled, and fourwalled CNTs with aspect ratios 9.1 and 4.51 obtained by Airebo potential [29] and Inclusion LJ with Rebo potential [11] differ from those of all of the other potentials due to layering effects of CNTs because in Airebo potential [29] and Inclusion LJ with Rebo potential [11], Van der Waals interaction is added which interact with interlayer carbon atoms during loading. Besides, From Tables 2 and 3, it is clearly observed that Young’s moduli, yield strengths, yield strains, ultimate strengths, and ultimate strains of singlewalled, doublewalled, threewalled, and fourwalled CNTs with aspect ratios 9.1 and 4.51 obtained by Rebo potential [31] and Airebo potential [29] differ from those of all of the other potentials due to torsional effects of C–C bonds of CNTs because, in Rebo potential [31] and Airebo potential [29], torsional interaction is added which include angular movement of C–C bond during loading.

From the tabular results, it is clearly observed that Young’s modulus of singlewalled, doublewalled, threewalled, and fourwalled CNTs with L/D ratios 9.1 and 4.51, respectively, obtained by Tersoff potential [10] is greater than that obtained by Rebo potential [11], Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29] because the slope of per atom potential energy with strain of CNTs obtained by Tersoff potential is higher than those of other potentials (see Figures 2 and 5). On the other hand, the ultimate strength of singlewalled, doublewalled, threewalled, and fourwalled CNTs with L/D ratios 9.1 and 4.51, respectively, obtained by Rebo potential [11] is greater than that obtained by Tersoff potential [10], Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29] because per atom potential energy of CNTs with strain obtained by Rebo potential is higher than those of other potentials and it takes the highest stress and strain to reach minimum per atom potential energy for the breaking of CNTs during tensile loading using Rebo potential [11] (see Figures 2 and 5). For single, double, three, and fourwalled CNTs, the ultimate strength obtained by Airebo [29] potential is lower than that of Rebo potential [11] because in Airebo potential [29] torsional and Van der Waals interactions are present which reduce per atom potential energy for which ultimate strength of CNTs obtained by Airebo potential [29] is lower as compared to Rebo potential [11]. For single, double, three, and fourwalled CNTs, the effects of torsion and Van der Waals interactions are observed clearly when their ultimate strength obtained by Rebo potential [11] is compared with that of Rebo potential [31], Inclusion LJ with Rebo potential [11], and Airebo potential [29]. From the tabular results, it is clear that torsion and Van der Waals interactions play an important role in their mechanical properties in the plastic range during loading.
When tensile load is applied at its both ends of CNTs using different potentials by molecular dynamics simulation, per atom potential energy decreases and during fracture per atom potential energy reaches a minimum value. As per atom potential energy of C–C structure using Tersoff potential is lower (Table in [33]) than that of Rebo potential [11] and Rebo potential [31], CNT will break at lower strain than that of other potentials and this phenomenon is already reflected in the above graphical and Tabular results. As bond radius and bond length of C–C in Tersoff potential are higher (see Table in [33]) than those of Rebo [11] and Rebo [31] potential, the stiffness of CNT and the slope of the stress strain curves using Tersoff potential should be higher than those of Rebo potential [11] and Rebo potential [31] and this phenomenon is clearly observed in the graphical and Tabular results. As per atom potential energy of C–C in Rebo potential [11] is higher (see Table in [33]) than that of Rebo [31] and Tersoff potential [10], the ultimate strength of CNT using Rebo potential [11] should be higher than that of Rebo [31] and Tersoff potential [10] because to reach minimum per atom potential energy for its breaking, it needs the highest tensile stress among all of the other potentials and from the graphical results, this phenomenon is also reflected in the graphical and tabular results. When Van der Waals interaction is present in Airebo potential [29], during tension some neighboring carbon atoms come in repulsive and attractive zone. As a result, C atoms experience extra stress during loading which enhance decreasing the ultimate strength of CNT. The other reason is that per atom potential energy of CNT structure obtained by Airebo potential [29] is lower than that of Rebo potential [11] and greater than that of Tersoff potential [10]. So for this reason, the ultimate strength of different types CNT using Airebo potential [29] is higher than that of Tersoff potential [10] and less than that of Rebo potential [11] which is reflected in the graphical and Tabular results.
From the tabular results as shown in Tables 2 and 3, the effects of layering, lengthtodiameter ratio of CNTs on their elastic, elasticplastic properties are clearly observed when the tension tests are carried out using different potentials. Besides, there is an observed effect of empirical potentials on Young’s modulus, yield strength, yield strain, ultimate strength, ultimate strain, and Poisson’s ratio of CNT under tension test using molecular dynamics simulation. Effects of potentials on the reliability and correctness of the solution are also reflected in the graphical and tabular results. Effects of layers and lengthtodiameter ratio of CNT are also reflected in the tabular results.
5. Conclusions
We study per atom potential energy of singlewalled CNT subjected to axial tensile load at its opposite ends at a very low strain rate using Rebo potential [11], Rebo potential [31], Airebo potential [29], and Tersoff potential [10]. We compare the stress strain relationship of singlewalled 1212 CNTs obtained by Rebo potential [11], Rebo potential [31], Airebo potential [29], and Tersoff potential [10] at a very low strain rate with that of Belytschko et al. [30] obtained by density functional theory and the stress strain relationship obtained by Rebo potential [11] and Airebo potential [29] agree with that of Belytschko et al. [30]. At high strain rate we also study the elastic, elasticplastic properties of single and multiwalled CNT subjected to uniform tension at its opposite ends using five different potentials such as Rebo potential [11], Rebo potential [31], Inclusion LJ with Rebo potential [11], Tersoff potential [10], and Airebo potential [29] with the published results as a comparative manner to understand the effect of potentials on the solution. From the comparative study it is clearly understood that the reliability and accuracy of Airebo potential [29] are higher than other potentials for the elastic, elasticplastic analysis of CNT because in Airebo potential [29] long range Van der Waals interaction and torsional effect of bond are included. To test the reliability of elastic, elasticplastic properties of CNTs obtained by us using different potentials, we compared our results with some published results and found out major limitations of such results which will be helpful for the further study of the elastic, elasticplastic properties of CNTs under tension. Effects of number of layers, lengthtodiameter ratio, and empirical potentials are also observed on the elastic, elasticplastic properties of CNTs.
Conflict of Interests
The authors declare that they have no conflict of interests regarding the publication of this paper.
References
 S. Lijima and T. Lchihashi, “Singleshell carbon nanotubes of 1nm diameter,” Nature, vol. 363, no. 6430, pp. 603–605, 1993. View at: Google Scholar
 D. S. Bethune, C. H. Kiang, M. S. De Vries et al., “Cobaltcatalysed growth of carbon nanotubes with singleatomiclayer walls,” Nature, vol. 363, no. 6430, pp. 605–607, 1993. View at: Google Scholar
 S. Iijima, “Helical microtubules of graphitic carbon,” Nature, vol. 354, no. 6348, pp. 56–58, 1991. View at: Google Scholar
 T. W. Ebbesen and P. M. Ajayan, “Largescale synthesis of carbon nanotubes,” Nature, vol. 358, no. 6383, pp. 220–222, 1992. View at: Google Scholar
 L. Merhari, Hybrid Nanocomposites for Nanotechnology: Electronic, Optical, Magnetic and Biomedical Applications, Springer, New York, NY, USA, 2009.
 O. Breuer and U. Sundararaj, “Big returns from small fibers: a review of polymer/carbon nanotube composites,” Polymer Composites, vol. 25, no. 6, pp. 630–645, 2004. View at: Publisher Site  Google Scholar
 B. I. Yakobson, C. J. Brabec, and J. Bernholc, “Nanomechanics of carbon tubes: instabilities beyond linear response,” Physical Review Letters, vol. 76, pp. 2511–2524, 1996. View at: Google Scholar
 A. Garg, J. Han, and S. B. Sinnott, “Interactions of carbonnanotubule proximal probe tips with diamond and graphene,” Physical Review Letters, vol. 81, no. 11, pp. 2260–2263, 1998. View at: Google Scholar
 B. I. Yakobson, M. P. Campbell, C. J. Brabec, and J. Bernholc, “High strain rate fracture and Cchain unraveling in carbon nanotubes,” Computational Materials Science, vol. 8, no. 4, pp. 341–348, 1997. View at: Google Scholar
 J. Tersoff, “New empirical approach for the structure and energy of covalent systems,” Physical Review B, vol. 37, no. 12, pp. 6991–7000, 1988. View at: Publisher Site  Google Scholar
 D. W. Brenner, “Empirical potential for hydrocarbons for use in simulating the chemical vapor deposition of diamond films,” Physical Review B, vol. 42, no. 15, pp. 9458–9471, 1990. View at: Publisher Site  Google Scholar
 S. B. Sinnott, O. A. Shenderova, C. T. White, and D. W. Brenner, “Mechanical properties of nanotubule fibers and composites determined from theoretical calculations and simulations,” Carbon, vol. 36, no. 12, pp. 1–9, 1998. View at: Google Scholar
 K. M. Liew, X. Q. He, and C. H. Wong, “On the study of elastic and plastic properties of multiwalled carbon nanotubes under axial tension using molecular dynamics simulation,” Acta Materialia, vol. 52, no. 9, pp. 2521–2527, 2004. View at: Publisher Site  Google Scholar
 P. M. Agrawal, B. S. Sudalayandi, L. M. Raff, and R. Komanduri, “Molecular dynamics (MD) simulations of the dependence of CC bond lengths and bond angles on the tensile strain in singlewall carbon nanotubes (SWCNT),” Computational Materials Science, vol. 41, no. 4, pp. 450–456, 2008. View at: Publisher Site  Google Scholar
 C. H. Wong and V. Vijayaraghavan, “Nanomechanics of imperfectly straight single walled carbon nanotubes under axial compression by using molecular dynamics simulation,” Computational Materials Science, vol. 53, no. 1, pp. 268–277, 2012. View at: Publisher Site  Google Scholar
 K. I. Tserpes and P. Papanikos, “Finite element modeling of singlewalled carbon nanotubes,” Composites Part B, vol. 36, no. 5, pp. 468–477, 2005. View at: Publisher Site  Google Scholar
 J.P. SalvetatDelmotte and A. Rubio, “Mechanical properties of carbon nanotubes: a fiber digest for beginners,” Carbon, vol. 40, no. 10, pp. 1729–1734, 2002. View at: Publisher Site  Google Scholar
 B. Coto, I. Antia, M. Blanco et al., “Molecular dynamics study of the influence of functionalization on the elastic properties of single and multiwall carbon nanotubes,” Computational Materials Science, vol. 50, no. 12, pp. 3417–3424, 2011. View at: Publisher Site  Google Scholar
 A. Mashreghi and M. M. Moshksar, “Bond lengths and bond angles of armchair singlewalled carbon nanotubes through molecular dynamics and potential energy curve approaches,” Computational Materials Science, vol. 49, no. 4, pp. 871–875, 2010. View at: Publisher Site  Google Scholar
 W. Tang, M. H. Santare, and S. G. Advani, “Melt processing and mechanical property characterization of multiwalled carbon nanotube/high density polyethylene (MWNT/HDPE) composite films,” Carbon, vol. 41, no. 14, pp. 2779–2785, 2003. View at: Publisher Site  Google Scholar
 M. Sammalkorpi, A. Krasheninnikov, A. Kuronen, K. Nordlund, and K. Kaski, “Mechanical properties of carbon nanotubes with vacancies and related defects,” Physical Review B, vol. 70, no. 24, Article ID 245416, 8 pages, 2005. View at: Publisher Site  Google Scholar
 Q. Wang, J. Dai, W. Li, Z. Wei, and J. Jiang, “The effects of CNT alignment on electrical conductivity and mechanical properties of SWNT/epoxy nanocomposites,” Composites Science and Technology, vol. 68, no. 78, pp. 1644–1648, 2008. View at: Publisher Site  Google Scholar
 A. Allaoui, S. Bai, H. M. Cheng, and J. B. Bai, “Mechanical and electrical properties of a MWNT/epoxy composite,” Composites Science and Technology, vol. 62, no. 15, pp. 1993–1998, 2002. View at: Publisher Site  Google Scholar
 J.P. Salvetat, J.M. Bonard, N. B. Thomson et al., “Mechanical properties of carbon nanotubes,” Applied Physics A, vol. 69, no. 3, pp. 255–260, 1999. View at: Publisher Site  Google Scholar
 Y. J. Liu and X. L. Chen, “Evaluations of the effective material properties of carbon nanotubebased composites using a nanoscale representative volume element,” Mechanics of Materials, vol. 35, no. 12, pp. 69–81, 2003. View at: Publisher Site  Google Scholar
 A. HernándezPérez and F. Avilés, “Modeling the influence of interphase on the elastic properties of carbon nanotube composites,” Computational Materials Science, vol. 47, no. 4, pp. 926–933, 2010. View at: Publisher Site  Google Scholar
 S. K. Deb Nath, H. Tohmyoh, and M. A. Salam Akanda, “Evaluation of elastic, elasticplastic properties of thin Pt wire by mechanical bending test,” Applied Physics A, vol. 103, no. 2, pp. 493–496, 2011. View at: Publisher Site  Google Scholar
 S. K. Deb Nath and S. G. Kim, “On the elastic, elasticplastic properties of Au nanowires in the range of diameters 1–200nm,” Journal of Applied Physics, vol. 112, no. 12, Article ID 123522, 10 pages, 2012. View at: Google Scholar
 S. J. Stuart, A. B. Tutein, and J. A. Harrison, “A reactive potential for hydrocarbons with intermolecular interactions,” Journal of Chemical Physics, vol. 112, no. 14, pp. 6472–6486, 2000. View at: Google Scholar
 T. Belytschko, S. P. Xiao, G. C. Schatz, and R. S. Ruoff, “Atomistic simulations of nanotube fracture,” Physical Review B, vol. 65, no. 23, Article ID 235430, 8 pages, 2002. View at: Google Scholar
 D. W. Brenner, O. A. Shenderova, J. A. Harrison, S. J. Stuart, B. Ni, and S. B. Sinnott, “A secondgeneration reactive empirical bond order (REBO) potential energy expression for hydrocarbons,” Journal of Physics: Condensed Matter, vol. 14, no. 4, pp. 783–802, 2002. View at: Publisher Site  Google Scholar
 W. H. Pres, B. P. Flannery, S. A. Teukoisky, and W. T. Vattering, Numerical Recipes, Cambridge University Press, Cambridge, UK, 1986.
 R. Smith and K. Beardmore, “Molecular dynamics studies of particle impacts with carbonbased materials,” Thin Solid Films, vol. 272, no. 2, pp. 255–270, 1996. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2014 S. K. Deb Nath and SungGaun Kim. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.